La0.1Ca0.9MnO3/Co3O4 for oxygen reduction and evolution reactions (ORER) in alkaline electrolyte
- 1.3k Downloads
Non-precious metal bifunctional catalysts are of great interest for metal–air batteries, electrolysis, and regenerative fuel cell systems due to their performance and cost benefits compared to the Pt group metals (PGM). In this work, metal oxides of La0.1Ca0.9MnO3 and nano Co3O47 catalyst as bifunctional catalysts were used in oxygen reduction and evolution reactions (ORER). The catalysts were characterized by X-ray diffraction (XRD), scanning electron microscopy (SEM), transmission electron microscopy (TEM), and N2 adsorption isotherms. The electrocatalytic activity of the perovskite-type La0.1Ca0.9MnO3 and Co3O4 catalysts both as single and mixtures of both were assessed in alkaline solutions at room temperature. Electrocatalyst activity, stability, and electrode kinetics were studied using cyclic voltammetry (CV) and rotating disk electrode (RDE). This study shows that the bifunctional performance of the mixed La0.1Ca0.9MnO3 and nano Co3O4 was superior in comparison to either La0.1Ca0.9MnO3 or nano Co3O4 alone for ORER. The improved activity is due to the synergistic effect between the La0.1Ca0.9MnO3 and nano Co3O4 structural and surface properties. This work illustrates that hybridization between these two metal oxides results in the excellent bifunctional oxygen redox activity, stability, and cyclability, leading to a cost-effective application in energy conversion and storage, albeit to the cost of higher catalyst loadings.
KeywordsAlkali electrolyte Bifunctional electrocatalyst Oxygen reduction Oxygen evolution Perovskite/spinel catalyst
Energy security and climate change are widely discussed due to the depletion of fossil fuels and adverse emissions produced while utilizing them. Currently, the energy demand and CO2 emission are 18 TW and 32 Gt year−1, respectively, and are predicted to reach 26 TW and 44 (55 total greenhouse gases (GHG)) Gt year−1 at 2040 [1, 2]. The GHG emissions are considered to be major contributors to the anthropogenic climate change. Ambitious targets were set by the recently signed Paris agreement (COP 21) to reduce global average temperature well below the 2 °C of preindustrial level in the twenty-first century . To achieve this target, further emission levels should be reduced and restricted to 40 Gt year−1 of GHG by 2030 . European Union has also set its own climate action plan for 80–95% reduction of GHG compared to the 1990 level. The EU has chosen the following sustainable means to meet the target: energy efficiency, renewable energy, nuclear energy, and carbon capture and storage (CCS). In particular, the renewable energy’s contribution to the total energy consumption is projected to increase from the current 10 to 50% by 2050 according to the high renewables scenario . The major important renewable energy sources are wind and solar and are projected to reach 26 and 11% of the total energy demand by 2050 [6, 7]. These two systems are intermittent and very much dependent on weather conditions. Therefore, their seamless integration into the grid for transmission to the end user requires a large-scale energy storage system. Currently, we are only able to store 1% of the total energy produced, and 98% of it accounts to gravitational energy stored through pumped water in hydroelectric plants. These are situated in high and low elevations, which in turn affect the social life and ecology of the sites . Electrochemical energy storage systems have attractive features such as modularity, scalability, fast response time, and high-energy efficiency, while they offer a wide range of energy and power densities, charge, discharge and life cycle, and capital cost .
Iron–air and Zn–air batteries in their early applications delivered energy densities up to 80 and 200 Wh kg−1 [10, 11]. The available iron and zinc reserves are 100 and 0.150 billion tons, respectively . They both use metals as negative electrodes and a bifunctional oxygen electrode as cathode. Oxygen redox reactions take place at the cathode which is the fundamental basis for a number of electrochemical systems such as metal–air batteries, fuel cells, and electrolyzers (water and chlor-alkali) [13, 14, 15, 16]. Even though the theoretical capacities of Fe and Zn electrodes, respectively, are 764 and 1080 mAh g−1, the capacities of the full cell comprising them are limited by the cathodic reactions at the positive electrode. Significant voltage losses arise during the charge and discharge reactions at the bifunctional air electrode due to the sluggish kinetics leading to significant overvoltages. In alkaline media, the oxygen reduction proceeds by two reaction pathways: (1) the direct 4e− and (2) the peroxide-mediated successive 2e−, followed by reduction and disproportionation or decomposition of the peroxide . The peroxide pathway is not desirable due to the corrosive species that affect the electrode materials and the active transition metal ions .
Some group of metals favor the direct 4e− pathway such as Pt group, pyrocholre, and perovskite families, whereas peroxide path is favored by carbon materials, Hg, Au, and most of the transition metals and oxides [18, 19]. The platinum group metals (PGM) such as Pt, RuO2, and IrO2 are regarded as state-of-the-art electrocatalysts for both the oxygen reduction reaction (ORR) and oxygen evolution reaction (OER) [20, 21, 22, 23, 24]. Although very low amount of PGM are currently incorporated in the electrode composites, they possess poor stability and their high cost due to limited availability hinders large-scale application and commercialization.
Perovskites with ABO3 structure have been considered as promising candidate electrocatalysts for the cathode, due to their bifunctionality, cost, availability, and stable performances in aqueous alkaline electrolytes. In ABO3, generally A belongs to rare-earth divalent ion (such as La, Ce, Nd, Sm, Gd, Dy, Yd, Ho, and Y) and alkaline earth elements (Ca and Sr) while B is a transition metal (Cr, Mn, Fe, Co, Ni, Cu). La-based perovskites outperform other A site elements due to it is high ionic size . Various perovskites have been developed such as LaCrO3, LaNiO3, LaMnO3, LaFeO3, and LaCoO3 [15, 19, 26]. Among them, Mn and Co-based perovskites have shown stable and high oxygen reduction and evolution reaction (ORER) performance due to their oxidation state and spin configuration. Bifunctional ORER performance of the perovskites follow a volcano-type curve, based on the occupancy of eg electronic state as primary activity descriptor, and electronegativity and spin state are considered as a secondary activity descriptor. eg electron occupancy < 1 is favored for ORR, and for OER, it should be eg > 1 [27, 28, 29]. Manganite-based perovskite’s oxidation state and eg electron filling vary from less than one to more than one based on A site and B site substitution. Altering the A and B sites results in interesting properties such as oxide ion mobility, electronic conductivity, and oxygen vacancies, which in turn augment the electrocatalytic properties on scale with or even better than PMG [30, 31]. Alkaline earth groups have similar ionic radii to lanthanides, are stable in high-temperature synthesis, and are low cost. Therefore, they are usually more or less substituted in place of the lanthanides. A site substitution results in increased current density and surface oxygen vacancies, conductivity, and stable crystal structure . B site cations affect the bond forming ability of B to oxygenated compounds. Several combinations of perovskite with Mn in the B site were studied such as La1 − xCa x MnO3, CaMnO3, and Ca2Mn2O5 . Their surface oxygen vacancies provide additional active sites for the oxygen redox activity. Ca2Mn2O5 (eg ≈ 1) has shown to have high OER performance, thanks to its molecular porosity and distorted structure . As mentioned above, Ca substitution results in mixed valence state of Mn (eg < 1), which consecutively produces oxygen vacancies by charge compensation and could promote the charge transfer and peroxide reduction . La1 − xCa x MnO3 has shown high conductivity and better bifunctional performance at even high porosity [35, 36]. In non-stoichiometric La0.1Ca0.9MnO3, Ca substitution results in increased amount of Mn4+ concentration, which in turn provides high conductivity and enhances the discharge performance comparable to MnO2 [16, 37, 38]. Though it has high ORR performance, its oxygen evolution performance has shown limitations.
Spinel Co3O4 is a low-cost magnetic p-type semiconductor with good structural stability and low environmental foot print and is commonly used in Li-ion battery, supercapacitor, solid-state sensors, heterogeneous catalyst, pigment, optical devices, photocatalyst, and oxygen evolution electrocatalyst [39, 40]. In recent years, there have been several studies reporting high OER activity with stable bifunctional performance of Co3O4 due to its mixed valance states [5, 41, 42, 43, 44, 45]. Although pure spinel itself is an efficient OER catalyst, its ORR performance is limited due to low conductivity and surface interaction. Recently, numerous strategies with complex or simple processes have been used for the preparation of Co3O4 showing substantial differences in size, shape, and surface properties for various applications [40, 45, 46, 47, 48, 49, 50]. There have been different co-catalysts mixed with Co3O4 to achieve high and stable bifunctional activity [44, 48, 51, 52, 53]. Partial substitution of the spinel Co3O4 tetrahedral sites with Ni, Mn, Cu, or Zn has resulted in improved performance, where the electronegativity of the dopant in the M–O bond tunes the catalytic properties. The electronegativity difference between Mn (1.55) and Co (1.80) is suggested to play important role in electron withdrawal and accepting properties [14, 54, 55, 56, 57]. More research effort has been centered on manganese and cobalt-based bifunctional catalysts, either alone or in mixture with other metals, due to their performance and abundance. MnO2–perovskite mixed catalysts have shown to perform well for bifunctional applications in alkaline electrolyte .
In this work, we prepared nanostructured Co3O4 through facile synthesis method at low temperatures by precipitation and aqueous phase oxidation and high surface area La0.1Ca0.9MnO3 through precipitation reaction, calcination, and followed at instant quenching. The oxide nanoparticles prepared with phase purity were characterized by XRD, SEM, TEM, and N2 adsorption isotherm. The electrochemical properties of the La0.1Ca0.9MnO3 and nano Co3O4 were investigated for their bifunctional activity and kinetics by cyclic voltammetry (CV) and linear sweep voltammetry (LSV) coupled with RDE. Single oxides as well as the combinations of the mixed oxides were for the first time studied for their OE and OR in order to evaluate their synergistic relationship for respective reactions and their stability in alkaline solutions.
Preparation of La0.1Ca0.9MnO3
All of the chemical reagents used for the preparation of the catalysts were of analytical grade and were applied without further purification. The perovskite La0.1Ca0.9MnO3 (LCMO) was prepared by the precipitation method using sodium carbonate as supporting electrolyte. The precursors of alkaline earth, rare earth, and transitional metals such as Ca, La, and Mn were all in hydrated forms of nitrates (VWR Chemicals) and were dissolved in distilled water in a molar ratio of 1:0.11:0.9 of respective salt and heated separately at 60 °C. Sodium carbonate solution (0.5 M) heated at 60 °C was slowly added to the aforementioned mixture kept in a bigger container, which was then stirred vigorously to ensue reaction by precipitation. After several steps of washing and decanting the supernatant, the precipitate was filtered off and dried at 120 °C for 12 h. The dry sample was then homogenized in a high-speed mixer and heat-treated at 700 °C in air for 6 h and was subjected to instant quenching in a water-cooled zone. The powder was then filtered and washed with deionized water followed by 5% acetic acid in order to remove any unreacted metal species and reduce its strong alkalinity. This step was again followed by drying and pulverization as a final step for the procurement of the catalyst.
Preparation of Co3O4
X-ray diffraction pattern was recorded by Siemens Diffractometer D5000, equipped with Ni-filtered Cu Kα radiation source (λ = 0.154 nm) at 40 kV and 30 mA in the 2θ range of 10°–80°. Phase identifications were done in EVA software, and corresponding powder diffraction file (PDF) numbers were reported. Scherrer’s equation was used on the XRD patterns to calculate the crystallite size. Specific surface area, pore volume, and pore size distributions were obtained by the multipoint Brunauer–Emmet–Teller (BET) analyses and by Barret–Joyner–Halenda method (BJH), respectively, using N2 adsorption isotherms (Micrometrics ASAP 2010) at a liquid N2 temperature. Prior to the analyses, the samples were degassed at 250 °C for 4 h. Zeiss Ultra-55 SEM and JEOL JEM-2100F TEM were used to analyze the particle sizes and their morphologies.
The composite electrodes had a gas diffusion layer, current collector, and the electrode material in a series of arrangement. They were prepared by mixing the electrode materials in the respective mass ratio (Table S1). The electrode composition was homogenized in a high-speed mixer at 6000 rpm (Waring® laboratory blender (LB20ES)) in the presence of hydrocarbon solvent (D-70® shellsol). After this, the filtered wet mass as active or catalyst layer was rolled on 100-mesh Ni wire screen on one side. The electrodes were pressed at 375 kg cm−2. Following this step, the electrode was dried in an oven to remove the solvent at 100 °C. The other side of the electrode was brush-painted by a solution containing 20 wt% PTFE (60 wt% dispersion) and continued until a uniform sealed layer on the nickel mesh was achieved to maintain a proper gas diffusion layer for supply or evolution of oxygen. The electrodes were then sintered in N2 atmosphere at 325 °C for 30 min . The final electrode dimensions were 3 × 5 cm, thickness 0.35 ± 0.05 mm with an active material loading of 6.5–34 mg cm−2 (Table S1) depending on the type and composition of the catalyst. The ratios of the oxide catalysts to graphite and PTFE were maintained at 4–5:1:1, except for the 20 wt% Pt/C, which had a ratio of 4:1 to PTFE.
The rotating disk electrode (RDE) experiment was performed on glassy carbon (GC) electrode (0.196 cm2). The RDE electrodes were prepared (Table S2) by ultrasonication (50 min) of the catalysts [LCMO, Co3O4, alone, or mixed together, 20 wt% Pt/C (ETEK) as a reference sample], graphite (Timrex HSAG 300, Timcal Ltd.), and 5 wt% Nafion as a binder having lower aliphatic alcohols and 3.6 g Milli-Q water with a resistivity of 18 MΩ and 0.4 g of isopropanol. The prepared ink 20 μl was drop-casted on the clean glassy carbon electrode and then dried.
The electrodes with bigger geometric area were tested in 6 M KOH (Sigma-Aldrich ACS reagent, ≥ 85%) in a three-electrode setup: composite electrode (working), Ni wire mesh (counter), and Hg/HgO (reference). The geometric area of 4 cm2 with the catalyst layer was immersed in the electrolyte, while the diffusion layer at the rear side was exposed towards the oxygen flow. The ORER activity was measured using CV in the potential range of − 0.35 to 0.70 V vs. Hg/HgO at the scan rate of 5 mV s−1.
In the RDE experiment, 1 M KOH as electrolyte prepared from Milli-Q water (18 MΩ cm) was used. Likewise, a three-electrode configuration was applied with the catalyst composite on the GC as a working electrode (see above), Pt ring mesh as counter electrode, and Hg/HgO in the same electrolyte as the reference electrode.
Here, j is the measured current density; j k and j d are the kinetic and diffusion limited current densities, respectively; ω is the rotation rate in rad s−1; n is the number of electrons transferred in the reaction; F is the Faraday constant (96,487 C mol−1); C O is the oxygen bulk concentration in 1 M KOH (7.8×10−7 mol cm−3); D O is the oxygen diffusion coefficient (1.8×10−5 cm2 s−1); υ is the kinematic viscosity (0.01 cm2 s−1) .
The CV and LSV measurements were conducted in SP-50 potentiostat (Biologic S.A., Claix, France). All the potential readings were measured against Hg/HgO reference electrode. The reported current densities were based on the geometric area of the corresponding electrode configuration. Current interrupt method was used to measure the internal resistance. The LSV recorded were automatically compensated for iR drop by the workstation.
Results and discussion
The morphology of the synthesized powders (LCMO and Co3O4) is shown in Fig. 1b, c. The TEM image (Fig. 1b) depicts that the high-temperature synthesis with subsequent quenching results in crystalline, small, and interconnected particles. Although porous structure increases the mass transfer by enabling the reactants to reach the active sites easily, the particles are closely packed, dominated by less internal cavities. However, the crystalline and interconnected particles may reduce the charge transfer resistance in the electrochemical reactions.
Most of the particles of the spinel Co3O4 are in cubic form uniformly distributed nanocrystals having mostly less than 30 nm in size, whereas very few of them exist in platelet nanoneedle-like morphology with less than 5 nm in diameter (Fig. 1c). The topotactic synthesis process of Co3O4 follows the reactions in Eqs. 1 and 2, where the sol-precipitation of the nanocrystals of Co(OH)2 is being transformed to nanowires according to Arhcer et al.  However, with vigorous stirring and longer reaction time by bubbling oxygen, oxidation of Co(OH)2 takes place through crystallization/deposition/growth, enabling the conversion to nanocubes with much less distinct oblong nanowires. Thus, the nanocubes of Co3O4 with the phase purity can be prepared without templates, additives, and/or thermal treatment, rendering small particle sizes as demonstrated from the line broadening of the diffractograms.
Surface properties of La0.1Ca0.9MnO3 and Co3O4
1. Surface area (m2 g−1)
2. Pore volume (cm3 g−1)
3. Average pore diameter (nm)
Figure 2b shows the voltammogram of Co3O4/graphite/Nafion electrode in N2-saturated 1 M KOH solution. In aqueous solutions following protonation and deprotonation, the cobalt oxides show two distinct redox pairs both at high and low potentials. During oxidation, peaks are observed at 0.26 and 0.56 V vs. Hg/HgO, respectively, with oxygen evolution to follow. The Co2+ starts oxidation prior to 0.26 V, and subsequently after 0.26 V, Co3+ is oxidized to Co4+. On the reverse scan, reversible peaks were observed at 0.52 and 0.2 V vs. Hg/HgO which are related to Co4+/Co3+ and Co3+/Co2+, respectively. The peaks attributed to the redox couple Co3+/Co4+ show a formal redox potential of 0.54 V vs. Hg/HgO [(Epa + Epc) / 2], having a peak potential difference of 40 mV in between, demonstrating a high amplitude and current density compared to the Co2+/Co3+ pair. Similar redox couples in alkaline electrolytes were also reported by Singh et al. , although preparation of the spinel, morphology, loading, type of support, electrolyte concentration, etc. might affect the small differences of the anodic potentials. The spinel Co3O4 (Co2+[Co+32] O4) has the mixed valence cobalt ion in its structure. These ions are progressively oxidized to produce both Co(III) and Co(IV) containing species as shown in Eqs. 5 and 6, which are catalytically supportive sites for the oxygen evolution reaction [66, 67]. The redox processes at the spinel Co3O4 proceeds through the following mechanism :
Co3O4 + OH− + H2O ⇄ 3CoOOH + e− (5) E0 = 0.222 V vs. Hg/HgO .
CoOOH + OH− ⇄ CoO2 + H2O + e− (6) E0 = 0.562 V vs. Hg/HgO .
Tafel slopes of OER and ORR
Slope (mV decade−1)
ORR low η
ORR high η
LCMO + Co3O4
In order to elucidate and determine the number of electrons exchanged and compare among the different catalysts prepared, Fig. S1a–d shows the RDE voltammograms for the compositions shown in Table S2. The RDE measurements were performed by linear sweep voltammetry mode at 2 mV s−1 with various rotation rates in O2-saturated 1 M KOH. This setup eliminates the mass transfer limitations and hence permitting us to investigate the kinetically controlled ORR. In all the catalysts, the limiting current densities (j L ) increased with the rotation rates, which is ascribed to the thinner diffusion layer that allows faster transport of oxygen to the electrode surface as function of the rotation rate. The polarization curves of the LCMO-based electrodes do possess bisigmoidal shapes.
Figure S1a shows the electrode containing LCMO catalyst polarization curve at different rotation rates, and the inset figure shows the Koutecky–Levich (K–L) plot. For the LCMO catalyst, the limiting current density (j L ) increased by twofold from 1.1 mA cm−2 when the rotation rate increased from 500 to 2500 rpm. Co3O4 (Fig. S1b) and LCMO + Co3O4 (Fig. S1c) electrodes exhibited lower current densities at the same rotation rate and potential. It is well known that without carbon support (high surface area carbon, reduced graphene oxide) and metal additives, pure Co3O4 having low conductivity shows low ORR activity [5, 44] as the graphite content is low in this study. The K–L plots (j−1 vs. ω−1) (inset in Fig. S1a–c) for all the three catalysts were parallel and linear at different potentials, which means that the ORR reaction follows the first-order kinetics. Figure S1d shows Pt polarization curves, which is a well-known catalyst for ORR. Its limiting current densities were much higher than the LCMO, Co3O4, and LCMO + Co3O4-based electrodes, and its K–L slopes at different potentials were near identical to each other compared to the well-separated curves of Fig. S1a–c.
The LCMO containing electrodes depicts pseudocapacitive rectangular current–voltage response, which are typical to multivalent Mn compounds. This capacitance arises due to the K+ and OH− ion electrosorption on the Mn ion oxygen vacancy sites . Figure 6a shows the voltammogram of the LCMO/graphite GDE. In the first cycle, LCMO exhibited high current densities corresponding to 29 and 59 mA cm−2 for the OER and ORR, respectively. After 50 cycles, the current densities for the OER and ORR of the same electrode dropped to 17 and 47 mA cm−2. On further charge and discharge cycles, the OER potential shifted to positive potential values, increasing by 80 mV from the initial 0.67 V vs. Hg/HgO. Thus, the current density for the OER was considerably decreased, while maintaining minor decline for the ORR, implying that the LCMO shows a higher activity for this later reaction. Figure 6b shows the voltammogram of the Co3O4/graphite/GDE. The first cycle delivered 61 and 8 mA cm−2 for OER and ORR, respectively. Upon successive cycles (10–50 cycles), the currents increased substantially for the OER and slightly for the ORR and were stabilized at 75 and 10 mA cm−2. This is a significant outcome, where both the oxygen evolution and reduction were shown to be enhanced by more than 20%, albeit the current density for the ORR was lower by more than a factor of 7 than for the OER.
The perovskite LCMO shown in Fig. 6a compared to spinel Co3O4 in Fig. 6b delivered high ORR current density, while on the other hand, Co3O4 has stable oxygen evolution performance. Therefore, combining the two catalysts has interesting features for the bifunctional OER/ORR, pertaining to their potential–current characteristics during the repeated cycles.
Figure 6c shows the voltammogram of the LCMO and Co3O4 mixed electrode performance. In the first cycle, the OE and OR current for the respective reactions was 58 and 45 mA cm−2, which were stabilized after 30 cycles and finally displayed at the 50th cycle at 48 and 37 mA cm−2. Remarkably, the ORER current densities were found to be still high and constant after the extended 50 cycles. The addition of Co3O4 resulted in the initial increase of the current density for OER by a factor of 2 compared to the LCMO-based GDE in Fig. 6a. However, the current density for the ORR was abated by about 0.8 times. The LCMO-based electrode showed a 41% current density decay from the 1st cycle to the 50th cycle in the OER direction, whereas addition of Co3O4 in these mixed oxide catalysts resulted in a 17% decrease. In the mixed LCMO and Co3O4, the electrode had 23 and 10 mg cm−2 for respective oxide catalyst, taken in separate mode but overall having 33 mg cm−2, whereas the loadings in the separately prepared LCMO and Co3O4-based electrodes were 34 and 32 mg cm−2, respectively. Though the amount of Co3O4 in the mixed type of electrode was lower than its corresponding single oxide electrode, the bifunctional performance hitherto shown supports the synergistic effects of LCMO and Co3O4 combined together. Although the ORR performance for many perovskites is considered to be low, La0.1Ca0.9MnO3 has shown to have a high catalytic activity for this reaction among the candidate perovskites studied and stable OER was noted for above 170 cycles for GDEs . The effects may be ascribed to the physicochemical nature of the perovskite and the synthesis method used. Furthermore, the enhancement of the OER may also be attributed to the nanoparticle sizes of the Co3O4, having high surface area and porous structure, prepared by the stepwise precipitation and oxidation.
Figure 6d presents the bifunctional activity of the commercial ETEK 20% Pt on Vulcan XC-72 electrode used as a benchmark to compare the electrode performance. Pt showed the highest oxygen reduction current (120 mA cm−2) among the catalysts studied during the first cycle, which then gradually increased to 152 mA cm−2. In addition, its OE performance was 16 mA cm−2 at the initial cycle, which then increased to 31 mA cm−2 at the 50th cycle. However, upon repeated cycles, the carbon support in the Pt-based electrode culminated in dissolution or corrosion turning the electrolyte into brownish color due to the high potentials (> 0.6 V vs. Hg/HgO) during the oxygen evolution. This phenomenon was not observed in the other catalytic materials as the support/conductive material was a high surface area graphite and its composition was four times lower than in the Pt-based electrode.
To further understand the electrodes’ morphological changes, scanning electron microscopy was performed at different magnifications on the fresh and on electrodes containing the catalysts LCMO + Co3O4, as well as Co3O4, and these are shown in Figs. S3 and S4. For comparison, SEM images of the constituent powder samples are also shown in Fig. S2. Figure S3 shows that the LCMO + Co3O4 electrode surface morphology at the initial stage (a, b) and after 50 cycles (c, d). After 50 cycles, Fig. S3c, d shows resemblance to the initial images in Fig. S3a, b without no significant change in both particle size and morphology. However, slight particle roughening was observed at higher magnification (Fig. S3d), which might be due to the presence of the KOH leading to crystals on the particles. Similar changes were also found on the only Co3O4 containing electrodes as shown in Fig. S4d. Overall, no major morphological changes were observed on these two samples, which might confirm that the catalysts were stable during the electrochemical cycling. Thus, the SEM together with the XRD results shows that the catalysts are structurally and crystallographically fit for the bifunctional activity of the OER/ORR during the length of the electrochemical operation.
The high activity of OER/ORR and durability of perovskite and Co3O4 mixed catalyst indicate that as a non-noble metal, earth-abundant and low-cost bifunctional catalyst can be used for application in metal–air batteries. The performance could be related to primarily eg (< 1) electron occupancy of the Mn ion (+ 3.7 and oxygen non-stoichiometry) and Co eg (> 1) mixed valence for the high OER and secondly the ionic conductivity of LCMO. These features make LCMO and Co3O4 mixed catalyst as an excellent catalyst for bifunctional catalyst for OER/ORR.
Co3O4-nanosized particles were synthesized successfully using a facile method. The resultant nanomaterials of both the spinel and the perovskite LCMO showed interconnected networks, having uniform particle size and high surface area with varied pore volumes and pore size distributions. The electrode kinetic studies of La0.1Ca0.9MnO3 mixed with Co3O4 showed improved bifunctional activity for both the ORR and OER. The spinel Co3O4 proceeds through the 2e− pathway, while La0.1Ca0.9MnO3 mixed with Co3O4 promotes a mixed pathway of both the 2e and 4e. Their bifunctional activity and stability in 6 M KOH on GDE showed that La0.1Ca0.9MnO3 mixed with Co3O4 showed durable and high performances compared to the single-phase electrodes of the respective catalysts. The OER mass activities were found to be similar on both the GC and GDE, although there are minor differences in the ORR due to operations and other physical parameters. The OER and ORR mass activities for the mixed catalyst were found to be 1.3 and 1.98 A g−1, respectively, exhibiting a quasi-reversible and effective catalytic response compared to similar single or mixed phase catalysts. The high activity of the mixed electrodes may be attributed to the structural robustness and synergistic effect. Ex situ XRD measurements of the cycled gas diffusion electrodes were shown to be structurally stable with no major phase transformation. The nanoblending and casting of two different catalysts such as in this study of the LCMO/Co3O4 may be considered as a strategy and a way forward for solving the high overpotentials encountered in both the OER/ORR and find applications in many electrochemical energy conversions and storage.
This work is supported by Swedish energy agency.
- 1.International Energy Agency, WEO (2015)Google Scholar
- 2.EMC (2015) The outlook for energy: a view to 2040Google Scholar
- 4.U. N secretariat. Paris Agreement, Decision 1/CP.21, Article 17Google Scholar
- 6.Technology Roadmap: Solar Photovoltaic Energy. (7 October 2014.). International Energy Agency (2014) “Technology Roadmap: Solar Photovoltaic Energy” (PDF) IEA Archived (PDF) from the original on 7 October 2014 Retrieved 7 October 2014Google Scholar
- 12.Narayanan SR, Prakash GKS, Manohar A, Yang B, Malkhandi S, Kindler A (2012) Materials challenges and technical approaches for realizing inexpensive and robust iron–air batteries for large-scale energy storage. Solid State Ionics 216:105–109. https://doi.org/10.1016/j.ssi.2011.12.002 CrossRefGoogle Scholar
- 14.Song W, Ren Z, Chen S-Y, Meng Y, Biswas S, Nandi P, Elsen HA, Gao P-X, Suib SL (2016) Ni- and Mn-promoted mesoporous Co3O4: a stable bifunctional catalyst with surface-structure-dependent activity for oxygen reduction reaction and oxygen evolution reaction. ACS Appl Mater Interfaces 8(32):20802–20813. https://doi.org/10.1021/acsami.6b06103 CrossRefGoogle Scholar
- 35.Celorrio V, Calvillo L, Dann E, Granozzi G, Aguadero A, Kramer D, Russell AE, Fermin DJ (2016) Oxygen reduction reaction at LaxCa1-xMnO3 nanostructures: interplay between A-site segregation and B-site valency. Catal Sci Technol 6(19):7231–7238. https://doi.org/10.1039/C6CY01105E CrossRefGoogle Scholar
- 41.Huang Y, Zhang M, Liu P, Wang L, Cheng F (2016) Improved performance of cobalt-based spinel by the simple solvothermal method as electrocatalyst for oxygen reduction reaction in alkaline solution. Ionics:1–8Google Scholar
- 42.Singh SK, Dhavale VM, Kurungot S (2015) Surface-tuned Co3O4 nanoparticles dispersed on nitrogen-doped graphene as an efficient cathode electrocatalyst for mechanical rechargeable zinc–air battery application. ACS Appl Mater Interfaces 7(38):21138–21149. https://doi.org/10.1021/acsami.5b04865 CrossRefGoogle Scholar
- 60.Qiao J, Xu L, Ding L, Shi P, Zhang L, Baker R, Zhang J (2013) Effect of KOH concentration on the oxygen reduction kinetics catalyzed by heat-treated co-pyridine/C electrocatalysts. Int J Electrochem Sci 8(1):1189–1208Google Scholar
- 64.Rascio DC, Souza RFBD, Teixeira Neto É, Suffredini HB, Santos MC, Calegaro ML (2010) Reaproveitamento de óxidos de manganês de pilhas descartadas para eletrocatálise da reação de redução de oxigênio em meio básico. Quím Nova 33(3):730–733. https://doi.org/10.1590/S0100-40422010000300043 CrossRefGoogle Scholar
- 65.Hamdani M, Singh R, Chartier P (2010) Co3O4 and Co-based spinel oxides bifunctional oxygen electrodes. Int J Electrochem Sci 5(4):556Google Scholar
- 68.Lyons ME, Brandon MP (2008) The oxygen evolution reaction on passive oxide covered transition metal electrodes in aqueous alkaline solution. Part 1-Nickel. Int J Electrochem Sci 3(12):1386–1424Google Scholar
- 70.Hosseini-Benhangi P, Garcia-Contreras MA, Alfantazi A, Gyenge EL (2015) Method for enhancing the bifunctional activity and durability of oxygen electrodes with mixed oxide Electrocatalysts: potential driven intercalation of potassium. J Electrochem Soc 162(12):F1356–F1366. https://doi.org/10.1149/2.0561512jes CrossRefGoogle Scholar
- 72.Thangasamy P, Selvakumar K, Sathish M, Kumar SMS, Thangamuthu R (2017) Anchoring of ultrafine Co3O4 nanoparticles on MWCNTs using supercritical fluid processing and its performance evaluation towards electrocatalytic oxygen reduction reaction. Catal Sci Technol 7(5):1227–1234. https://doi.org/10.1039/C6CY02611G CrossRefGoogle Scholar
- 75.Malkhandi S, Trinh P, Manohar AK, Jayachandrababu KC, Kindler A, Surya Prakash GK, Narayanan SR (2013) Electrocatalytic activity of transition metal oxide-carbon composites for oxygen reduction in alkaline batteries and fuel cells. J Electrochem Soc 160(9):F943–F952. https://doi.org/10.1149/2.109308jes CrossRefGoogle Scholar
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.